Effects of sintering parameters on the microstructure and tensile
Embed Size (px)
Transcript of Effects of sintering parameters on the microstructure and tensile
Materials and Design 32 (2011) 33473353
Contents lists available at ScienceDirect
Materials and Design
journal homepage: www.elsevier .com/locate /matdes
Effects of sintering parameters on the microstructure and tensile properties of in situTiBw/Ti6Al4V composites with a novel network architecture
L.J. Huang a, L. Geng a,, H.X. Peng b, K. Balasubramaniam a, G.S. Wang aa School of Materials Science and Engineering, Harbin Institute of Technology, P.O. Box 433, Harbin 150001, Chinab Advanced Composites Centre for Innovation and Science (ACCIS), Bristol University, Bristol, BS8 1TR, United Kingdom
a r t i c l e i n f o a b s t r a c t
Article history:Received 26 November 2010Accepted 5 February 2011Available online 12 February 2011
Keywords:A. Metal matrix compositesC. Powder metallurgyF. Microstructure
0261-3069/$ - see front matter 2011 Elsevier Ltd. Adoi:10.1016/j.matdes.2011.02.023
Corresponding author. Tel.: +86 451 86418836; faE-mail addresses: email@example.com (L.J. H
com, firstname.lastname@example.org (L. Geng).
In order to better understand the relationship of processingstructuremechanical properties of in situTiB whisker reinforced Ti6Al4V (TiBw/Ti64) composites with a novel network architecture, the effectsof sintering parameters on the microstructure and tensile properties of the composites were investigated.TiB whiskers with the highest aspect ratio and the coarsest whiskers were obtained at 1100 C and1200 C due to the skips of whisker growth speeds along the [0 1 0] direction and the [0 0 1] and[1 0 0] directions, respectively. Additionally, TiB whisker with a claw-like structure can be synthesizedfrom one TiB2 polycrystal parent. The quasi-continuous network architecture of TiBw/Ti64 compositescan be achieved at higher sintering temperatures more than 1200 C. The prepared composites withthe quasi-continuous network architecture exhibit a superior combination of tensile properties.
2011 Elsevier Ltd. All rights reserved.
Titanium matrix composites (TMCs) attract much more attentiondue to their high special strength, high special stiffness, excellentwear resistance and high temperature durability, which renderthem as the optimal candidate material for a range of commercialautomotive, aerospace and military applications [1,2]. TMCs canbe divided into the continuous fiber reinforced titanium matrixcomposites (CRTMCs)  and the discontinuous particle and/orwhisker reinforced titanium matrix composites (DRTMCs) [4,5].Furthermore, the discontinuous TiB whiskers and/or TiC particles[1,2,6] reinforced titanium matrix composites fabricated by in situmethods are sought-after due to their superior and isotropic proper-ties and low cost. Moreover, TiB whiskers are regarded as theoptimal reinforcement not only because of its high modulus andhardness and good chemical compatibility with Ti matrix but alsoits similar density and thermal expansion coefficient with Ti matrix[2,7]. Powder metallurgy (PM) process, one of in situ methods, hasbeen considered to be an excellent method to fabricate TMCs largelydue to its ability for microstructural control, near net shape process-ing, minimal material waste and low cost .
Irrespective of the method and reinforcement used, the aim isalways to obtain a homogeneous reinforcement distribution wherethe reinforcements are uniformly dispersed in titanium matrix[2,7,9]. However, many TMCs with the homogeneous microstruc-
ll rights reserved.
x: +86 451 86413922.uang), genglingroup@gmail.
ture exhibit a limited improvement of mechanical properties, eveninferior mechanical properties such as extreme brittleness forTMCs fabricated by the conventional PM processes including highenergy milling, isostatic cool pressing, sintering and extrusion[2,7,8].
Fortunately, it was well demonstrated that the serious draw-backs have been solved by tailoring a novel network reinforcementdistribution of TiBw/Ti64 composites fabricated by a simplified PMprocess in our previous work . Not only TMCs with the networkmicrostructure exhibited a superior combination of properties, butalso the fabrication processes were significantly simplified byusing the low-energy milling and one-step sintering processeswithout any subsequent treatment such as extrusion. On the onehand, different raw materials require different sintering parame-ters, and on the other hand, the formation mechanism of branchedand dowel-like TiBw structures which can exploit a betterstrengthening effect has not been reported up to now. Therefore,it is certainly interesting and important to investigate the effectsof sintering parameters on the microstructure (the nucleationand growth of TiB whisker) and tensile properties of in situ TiBw/Ti64 composites with a novel network microstructure.
2. Experimental procedure
The spherical Ti64 powders with a large size of 180220 lm(Fig. 1a), prismatic TiB2 powders with a small size of 18 lm(Fig. 1b) were selected in the present study in order to obtain thenetwork reinforcement architecture. The chemical composition of
http://dx.doi.org/10.1016/j.matdes.2011.02.023mailto:email@example.com:genglingroup@gmail. commailto:genglingroup@gmail. commailto:firstname.lastname@example.org://dx.doi.org/10.1016/j.matdes.2011.02.023http://www.sciencedirect.com/science/journal/02613069http://www.elsevier.com/locate/matdes
Fig. 1. Flow chart of fabrication of TiBw/Ti64 composites with a network microstructure and SEM micrographs of raw materials and the mixture: (a) Ti64 powder (180220 lm), (b) TiB2 powder (18 lm), (c) the mixture of Ti64 and TiB2, and (d) schematic illustration showing that TiB2 powders were adhered onto the surface of Ti64 powder.
3348 L.J. Huang et al. / Materials and Design 32 (2011) 33473353
the selected Ti64 powders (in wt.%) is 6.42Al, 4.12 V, 0.16Fe, 0.12O,0.024Si, 0.028 others, and balance titanium.
The large Ti64 and small TiB2 powders were low-energy milledat a low speed of 200 rpm for a period of 8hrs. The fine TiB2 pow-ders adhered onto the surface of the large Ti64 particles by thesimplified low-energy milling process as shown in Fig. 1c and d.All the milling processes were carried out under a protective argonatmosphere. To obtain the optimal fabrication parameters and fur-ther explore the effects of sintering temperature and holding timeon the microstructure and mechanical properties of TMCs with anetwork microstructure, a range of TiBw/Ti64 composites werefabricated at 1000 C, 1100 C, 1200 C and 1300 C for a constantholding time of 1.0 h, and another two were fabricated at a con-stant sintering temperature of 1200 C but for different holdingtimes of 0.5 h and 1.5 h, respectively. Then the blended mixtureswere hot pressed in vacuum (102 Pa) under a pressure of20 MPa at the different sintering temperatures (1000 C, 1100 C,1200 C and 1300 C) and for different times (0.5 h, 1.0 h and1.5 h) according to the above design. TiB whiskers can be synthe-sized according to the following reaction equation:
Ti TiB2 ! 2TiB 1
The nominal volume fraction of TiBw reinforcement in all theTMCs is 5 vol.%. T1000t1.0, T1100t1.0, T1200t1.0 and T1300t1.0 are repre-sented as the 5 vol.%TiBw/Ti64 composites fabricated at 1000 C,1100 C, 1200 C and 1300 C, respectively, for a constant holdingtime of 1.0 h, and T1200t0.5 and T1200t1.5 are represented as the
5 vol.%TiBw/Ti64 composites fabricated at 1200 C but for differentholding times of 0.5 and 1.5 h, respectively. These signs are alsolisted in Table 1. T represents the sintering temperature while tthe holding time.
Tensile tests were carried out using an Instron-5569 universaltesting machine at a constant crosshead speed of 0.5 mm/min. Ten-sile specimens have gauge dimensions of 15 mm 5 mm 2 mmand a total of five specimens were tested for each material. Micro-structural examination was performed using a scanning electronmicroscope (SEM, Hitachi S-4700).
3. Results and discussions
Fig. 2 shows a network morphology of reinforcement distribu-tion in the 5 vol.%TiBw/Ti64 composites fabricated at the lowesttemperature (1000 C, Fig. 2a) and the highest temperature(1300 C, Fig. 2b), respectively. It is quite obvious that many poreswhich are large in size retain while fabricating the composite at thelowest temperature (1000 C) as shown in the insert image ofFig. 2a). However, increasing the sintering temperature up to1300 C can totally eliminate these pores and form a compact com-posite as shown in Fig. 2b. On the one hand, increasing tempera-ture softens the Ti64 matrix, and on the other hand, moreadequate exothermic reactions of Ti and TiB2 at the highest
Table 1Tensile properties of in situ 5 vol.%TiBw/Ti64 composites fabricated by different sintering parameters.
Sintering temperature (C) Holding time (h) Yield strength (MPa) Ultimate strength (MPa) Elongation (%) Elastic modulus (GPa)
1000 1.0 318 7 117.3 0.51100 736 5 122.1 0.51200 970 6 1112 6 3.0 0.5 123.1 0.61300 973 5 1101 7 2.8 0.41200 0.5 969 4 1116 5 2.5 0.6
1.5 976 5 1120 8 2.7 0.5
Fig. 2. SEM micrographs of 5 vol.%TiBw/Ti64 composites with a novel network microstructure fabricated at (a) 1000 C and (b) 1300 C by hot pressing reaction.
L.J. Huang et al. / Materials and Design 32 (2011) 33473353 3349
temperature further softens the local matrix. The above two factorslargely decrease the resistance of hot deformation to form thecompact composite. Additionally, it can be clearly seen fromFig. 2 that the width of the TiBw reinforcement network, namelyTiBw length, of the composite fabricated at 1300 C is obviouslywider than that of the composite fabricated at 1000 C. The reasonis that the diffusion distance and speed of B element can be largelyincreased with increasing the